Water Oxidation Catalysis by [email protected]
Oxide Core−Shell Nanocomposites Gökhan Elmaci,† Carolin E. Frey,‡ Philipp Kurz,*,‡ and Birgül Zümreoğlu-Karan*,† †
Chemistry Department, Hacettepe University, Beytepe Campus, 06800 Ankara, Turkey Institut für Anorganische und Analytische Chemie, Albert-Ludwigs-Universität Freiburg, Albertstraße 21, 79104 Freiburg, Germany
S Supporting Information *
ABSTRACT: In this work, magnetic nanocomposite particles were prepared for water oxidation reactions. The studied catalysts consist of maghemite (γ-Fe2O3), magnetite (Fe3O4), and manganese ferrite (MnFe2O4) nanoparticles as cores coated in situ with birnessite-type manganese oxide shells and were characterized by X-ray diﬀraction, transmission electron microscopy, scanning electron microscopy, thermal, chemical, and surface analyses, and magnetic measurements. The particles were found to be of nearly spherical core−shell architectures with average diameter of 150 nm. Water oxidation catalysis was examined using Ce4+ as the sacriﬁcial oxidant. All core− shell particles were found to be active water oxidation catalysts. However, the activity was found to depend on a variety of factors like the type of iron oxide core, the structure and composition of the shell, the coating characteristics, and the surface properties. Catalysts containing magnetite and manganese ferrite as core materials displayed higher catalytic activities per manganese ion (2650 or 3150 mmolO2 molMn−1 h−1) or per mass than nanoiron oxides (no activity) or birnessite alone (1850 mmolO2 molMn−1 h−1). This indicates synergistic eﬀects between the MnOx shell and the FeOx core of the composites and proves the potential of the presented core−shell approach for further catalyst optimization. Additionally, the FeOx cores of the particles allow magnetic recovery of the catalyst and might also be beneﬁcial for applications in water-oxidizing anodes because the incorporation of iron might enhance the overall conductivity of the material.
INTRODUCTION As a solution to the worldwide energy demand, hydrogen holds promise as a clean energy carrier. Water splitting using renewable energy sources is a very attractive concept to generate molecular hydrogen from water as a “sustainable fuel”. However, the overall water-splitting reaction requires water oxidation as one of the half-reactions, which is electrochemically diﬃcult and thus often requires high overvoltages.1 Many current scientiﬁc eﬀorts therefore focus on the development of new materials for catalysis of the water oxidation process. In this ﬁeld, manganese-based systems are of particular interest because they mimic the role of manganese in biological water oxidation (Photosystem II).2 Additionally, manganese is available on a large scale because of the abundance of manganese minerals. Various manganese compounds have been given signiﬁcant attention as water oxidation catalysts in chemical, photochemical, and/or electrochemical systems.3 Among the homogeneous systems reported, mono- and polynuclear manganese complexes showed only low catalytic rates and stabilities4,5 but displayed better performances when adsorbed on clay or Naﬁon matrixes.6−8 Compared to these molecular catalysts, manganese oxides are thermodynamically more stable. Early experiments already demonstrated that manganese(III) © XXXX American Chemical Society
oxides or hydroxides are able to catalyze the oxidation of water in the presence of (photo)chemical oxidants such as Ce4+ or [Ru(bpy)3]3+ although only with low reaction rates.9,10 Recent studies indicated that the incorporation of Ca2+ into the manganese oxide structure enhances the catalytic activity signiﬁcantly.11−13 X-ray diﬀraction and absorption studies revealed that these catalysts are materials of low crystallinity composed of layers of edge-sharing MnO6 octahedra with interlayer Ca2+ ions. The manganese ions show an average oxidation state of about +3.8, and overall the materials resemble the birnessite type of manganese oxide minerals.14,15 Over the last years, birnessites have been closely investigated as catalysts for water oxidation.15−17 Both performance enhancement by adding Ca2+ and by controlling the particle morphology seem to be of importance because nanosized CaMnOx particles proved to be more eﬃcient catalysts than binary manganese oxides (Mn3O4, Mn2O3, and MnO2) of similar size.18 In this contribution, we follow the track of morphology control and report on ∼150 nm small, magnetic [email protected]
composite catalyst particles, which were prepared by in situ Received: December 5, 2014
DOI: 10.1021/ic502908w Inorg. Chem. XXXX, XXX, XXX−XXX
Water Oxidation Catalysis Using Ce4+ as the Chemical Oxidant. Precisely weighed particle samples (about 5 mg each) and 685 mg (1.25 mmol) of ammonium cerium(IV) nitrate [(NH4)2Ce(NO3)6] were ﬁlled into 20 mL septum vials. After the addition of 5 mL of air-saturated water, the vials were capped immediately using gastight septa and sonicated for 20 s. The reaction containers were now kept at 40 °C in a water bath, and headspace gas samples (100 μL each) were taken from the vials at 10 min intervals using a gastight syringe (Hamilton). The gas samples were injected into a PerkinElmer Clarus 480 gas chromatograph equipped with a 12 ft × 1/8 in., 5 Å molecular sieve column (Restek) and a thermal conductivity detector. Six injections at 10 min intervals were carried out. The amount of evolved oxygen was then calculated for each headspace extraction from the detected oxygen/nitrogen signal ratios. To do so, the amount of oxygen from air (corresponding to the detected nitrogen peak) was calculated and subtracted, leaving excess oxygen generated by the water oxidation reaction. For further details concerning the methodology of the water oxidation catalysis runs used here, refer to ref 13.
coating of manganese ferrite (MF), magnetite (MG), and maghemite (MH) nanoparticles serving as template cores with birnessite-type manganese oxide (B) shells. The resulting nanocomposites show promising activities in water oxidation catalysis. Additionally, the materials’ magnetic properties allow a practical recovery of the catalysts by applying an external ﬁeld, and the core−shell architecture might be a useful concept to inﬂuence the electronic conductivity, a key parameter for use of the materials as electrocatalysts.
Materials. The core materials γ-Fe2O3 (Sigma, nanopowder of